- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Recently Accepted Articles ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Advances in Materials Science and Engineering

Volume 2013 (2013), Article ID 950439, 5 pages

http://dx.doi.org/10.1155/2013/950439

## Surface State Capture Cross-Section at the Interface between Silicon and Hafnium Oxide

Department of Electronic Engineering, Ming Chuan University, Taoyuan, Taiwan 333, Taiwan

Received 5 August 2013; Accepted 30 September 2013

Academic Editor: Chun-Hsing Shih

Copyright © 2013 Fu-Chien Chiu. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The interfacial properties between silicon and hafnium oxide (HfO_{2}) are explored by the gated-diode method and the subthreshold measurement. The density of interface-trapped charges, the current induced by surface defect centers, the surface recombination velocity, and the surface state capture cross-section are obtained in this work. Among the interfacial properties, the surface state capture cross-section is approximately constant even if the postdeposition annealing condition is changed. This effective capture cross-section of surface states is about 2.4 × 10^{−15} cm^{2}, which may be an inherent nature in the HfO_{2}/Si interface.

#### 1. Introduction

Hafnium oxide (HfO_{2}) has emerged recently as an essential dielectric material in the semiconductor industry, currently being used in logic gate stacks [1] and considered a promising candidate for resistance switching memory devices [2, 3] as well as surface passivation of advanced Si solar cells [4, 5]. Therefore, the determination of surface state capture cross-section at the interface between silicon and hafnium oxide is of great importance for the semiconductor industry, the photovoltaic industry, and the scientific community. The known characteristics of HfO_{2} thin films include a large band gap (~6 eV) [6], a relatively high dielectric constant (>20) [7], an acceptable breakdown strength (>4 MV/cm) [7], excellent thermodynamic stability [8], and an effective mass of carrier transportation [9]. In this work, the interface characteristics of the interface-trapped charge density (), the interface-trapped charge density per area and energy (), the effective capture cross-section () of surface states, the surface recombination velocity (), and the minority carrier lifetime () are identified. The typically electrical measurements of current-voltage () and capacitance-voltage () characteristics were performed on the Al/HfO_{2}/p-Si metal-oxide-semiconductor (MOS) capacitors and metal-oxide-semiconductor field-effect transistors (MOSFETs). Both gated-diode method [10, 11] and subthreshold measurement [12] were applied to evaluate the capture cross-section of interface states for the HfO_{2}-gated MOSFETs. The gated-diode method is a simple way to accurately identify the interfacial characteristics using only a sweeping dc gate voltage, which was introduced in 1966 by Grove and Fitzgerald [10] to determine the surface-state density in MOS structures. According to the gated-diode measurements, the surface recombination velocity and the minority carrier lifetime () in the field-induced depletion region were extracted. In addition, the interface-trapped charge density per area and energy () was determined by using the device subthreshold measurement. Consequently, the effective capture cross-section of surface states was determined to be about 2.4 × 10^{−15} cm^{2} by the combination of gated-diode and device subthreshold measurements.

#### 2. Experiment

Here, (100) -type silicon wafers (1–5 Ω-cm) were used as the starting material. Following the standard cleaning procedures, a 500 nm SiO_{2} film was grown on silicon wafers by wet oxidation. The source and drain windows were defined by wet etching and doped by phosphorous diffusion. The HfO_{2} films were deposited by RF magnetron sputtering in argon ambient at room temperature. The flow rate of argon was 13.5 standard cubic centimeters per minute (sccm). The total pressure during deposition was 20 mtorr. The refractive index, energy bandgap, and thickness of these thin films were measured by an N&K analyzer. The optical refractive index () and energy bandgap () were around 1.9–2.1 and 5.6–5.8 eV, respectively. The deposited thicknesses of HfO_{2} thin films ranged from 12 nm to 47.1 nm. After HfO_{2} deposition, the postdeposition anneal (PDA) was performed in either N_{2} or N_{2}/O_{2} (i.e., 50% N_{2} and 50% O_{2}) with a flow rate of 3 sccm for 60 s at 500°C. According to the X-ray diffraction analysis, the HfO_{2} films annealed at 500°C were amorphous. The aluminum (Al) electrodes were evaporated and patterned using a wet etching process. Postmetallization annealing (PMA) was performed at 400°C in N_{2} for 30 s. The Al/HfO_{2}/-Si MOS capacitors and MOSFETs were measured by Agilent 4156C semiconductor parameter analyzer and Agilent 4284A impedance analyzer. All the measurements were performed under dark condition. Based on the high-frequency (1 MHz) measurements for the MOS capacitors, the effective dielectric constant of HfO_{2} films annealed at 500°C in N_{2} or N_{2}/O_{2} was evaluated as 18.9 or 19.3, respectively (not shown here). In this work, the relatively large devices were chosen to avoid the short channel effects which may cause the distortion in analysis of surface state capture cross-section. The channel width () is 100 *μ*m and the channel length () is 19 *μ*m.

#### 3. Results and Discussion

The drastic irregularity of the oxide/Si interface should introduce a large amount of density of states into the forbidden gap near the interface. The interface state may cause the charge trapping and lead to the device instability as well as the degradation of subthreshold swing, off-state current, carrier mobility, and oxide reliability. Charge carriers can be trapped or captured while they come to the physical vicinity of the center of the interface state. The capture cross-section () of the center is a measure of how close the carrier has to come to the center to be captured. In this work, the gated-diode method is used to identify the interface-trapped charge density (), the surface recombination velocity (), and the minority carrier lifetime () in the field-induced depletion region for the nMOSFET devices using HfO_{2} gate dielectrics annealed at 500°C. The test structure described by Grove and Fitzgerald to investigate surface properties in MOS structures is identical to a MOSFET without or with an unconnected source region. In this work, the gated-diode measurement was made using a floating source and a grounded substrate on MOSFET structures, as shown in Figure 1(a). The drain is reversely biased with respect to the substrate (). According to the theory of gated-diode method, the reverse current of junctions () is a function of the gate bias (). The - characteristics may exhibit three distinct regions [10], as indicated in Figure 1(b). The reverse current of junctions comes from the generation of electron-hole pairs at generation-recombination centers in the depletion region at room temperature. Hence, the magnitude of reverse current depends on the density of such centers and the volume of the depletion region. As the volume of the depletion region in gated diodes depends on the gate voltage, reverse current also depends on the gate voltage. The HfO_{2}/silicon interface is in the accumulation mode when is less than the flat band voltage , and the reverse diode current originates from the generation-recombination centers in the depletion region of the metallurgical junction (). When (where is the threshold voltage), the field-induced junction is depleted, and the rapid increase in the reverse diode current is caused by the generation of electron-hole pairs at the generation-combination centers of the surface region () and the field-induced junction depletion region (). At , the field-induced junction is in the inversion mode and the reverse diode current is reduced by the filling of the interface-trapped charge states by the minority carriers. The magnitude of the reverse diode current is the sum of the generation currents in the depletion volume of the field-induced junction and in that of the metallurgical junction. Based on the Shockley-Read-Hall theory for the single-level centers [10], the equations for the gated-diode are written as follows [13–15]:
where cm^{−3} is the intrinsic carrier concentration in silicon [12]; represents the area of the metallurgical junction; cm^{−2} is the gate area; is the surface recombination velocity; is the effective capture cross-section area; = 10^{7} cm/s is the thermal velocity; is the built-in potential of the junction; is the quasi-Fermi potential of the majority carriers of the substrate; is the width of the depletion region of the metallurgical junction; is the maximum width of the surface depletion region; is the minority carrier lifetime in the field-induced depletion region; is the interface-trapped charge density (i.e., density of the single-level surface generation-recombination centers per unit area); is the interface-trapped charge density per area and energy (i.e., the density of uniformly distributed surface generation-recombination centers per unit area and energy); and , , and are the generation and recombination rates of carriers per unit volume in the depletion regions of the metallurgical, the surface region, and field-induced region, respectively.

Figure 2 shows the reverse diode current versus for the HfO_{2} gated-diodes at V. Through the gated diode method, the surface recombination velocity () and the minority carrier lifetime () in the field-induced depletion region can be extracted. For HfO_{2} films annealed in N_{2}/O_{2}, and are determined to be 4.1 × 10^{3} cm/s and 16 ns. On the other hand, for HfO_{2} films annealed in N_{2}, and are determined to be 8.9 × 10^{3} cm/s and 22 ns. Obviously, the reverse diode current of nMOSFETs for HfO_{2} annealed at 500°C in N_{2}/O_{2} is smaller than that annealed in N_{2}. The reduction in reverse current may be attributed to the decrease in oxygen vacancy related defects [16–19] in HfO_{2}. The oxygen vacancy is one type of trapping centers and is easily formed in HfO_{2} due to the transportation of oxygen atoms from HfO_{2} into Si [18, 19]. During the thermal treatment of PDA in N_{2}/O_{2} ambient, the oxygen atoms can diffuse into the HfO_{2} films to partially passivate the existing oxygen vacancies. Hence, the reverse diode current can be reduced by N_{2}/O_{2} annealing.

Figure 3 shows the characteristics. The ratio is larger than 10^{6} at V, indicating that the nMOSFETs with amorphous HfO_{2} gate dielectrics have a good current switch capability. The subthreshold swings () for the HfO_{2} gate dielectrics annealed at 500°C in N_{2} and N_{2}/O_{2} are about 85.1 and 76.4 mV/dec, respectively. According to Figure 3, the density of interface traps per area and energy () can be determined from the subthreshold swing measurement, because is expressed as [12], where is the depletion-layer capacitance, is the capacitance associated with the interface traps, and is the dielectric capacitance. The determined is about 4.6 × 10^{12} and 2.1 × 10^{12} cm^{−2}-eV^{−1} for HfO_{2} annealed at 500°C in N_{2} and N_{2}/O_{2}, respectively. Once is determined, and can be extracted using (4). For HfO_{2} annealed in N_{2}, and are extracted to be about 2.4 × 10^{−15} cm^{2} and 3.7 × 10^{11} cm^{−2}, respectively; for HfO_{2} annealed in N_{2}/O_{2}, and are extracted to be 2.4 × 10^{−15} cm^{2} and 1.7 × 10^{11} cm^{−2}, respectively. It is worthy of note that the same value is obtained for HfO_{2} annealed both in N_{2} and in N_{2}/O_{2}. This finding may imply that the capture cross-section of surface states is an inherent nature at the HfO_{2}/Si interface. The universal constant of surface state capture cross-section is around 2.4 × 10^{−15} cm^{2}.

Figure 4 shows the channel electron mobility versus the effective electric field. The effective surface field () and effective channel mobility () can be expressed as and , respectively, where is the inversion layer charge, is the bulk depletion layer charge, and is the dielectric constant of Si. The linear approximation of , , is used in evaluating the mobility. The rest of the symbols have been defined earlier. The maximum channel electron mobility for the HfO_{2} annealed in N_{2}/O_{2} and N_{2} was determined to be 102 and 43 cm^{2}/V s, respectively. Evidently the HfO_{2} film annealed in N_{2} shows lower channel electron mobility than the film annealed in N_{2}/O_{2} condition. In addition, the HfO_{2} device has a lowered mobility as compared to a universal mobility curve in SiO_{2} MOSFETs [20]. The lowered mobility may come from the larger surface states which cause the increased interface charge scattering [21].

Table 1 lists the capture cross-sections of surface states () at the interface between silicon and oxides, for example, SiO_{2}, ZrO_{2}, Al_{2}O_{3}, CeO_{2}, and HfO_{2} [22–29]. For SiO_{2}, the value is 1–4 × 10^{−16} cm^{2} [22–24] which is smaller than those of high-k dielectrics. For CeO_{2}, the value is around 9 × 10^{−15} cm^{2} even if the adopted measurement method is different [27, 28]. In this work, the experimental results show that the HfO_{2} films annealed in N_{2}/O_{2} have lower interface state density () and higher channel electron mobility () compared to the HfO_{2} films annealed in N_{2}. Although the different PDA conditions lead to the different values of and , the same for HfO_{2} deposited by rf magnetron sputtering is obtained to be around 2.4 × 10^{−15} cm^{2}. This finding may suggest that the capture cross-section of surface states for some thin film deposition method may be an inherent nature at the interface between silicon and hafnium oxide. It is worthy to note that the capture cross-section of surface states may be influenced by the factors of environment temperature, film thickness, film deposition method, and especially surface preparation of Si substrate prior to HfO_{2} deposition.

#### 4. Conclusions

The electrical properties at the HfO_{2}/Si interface are investigated by the gated-diode method and the subthreshold measurement. Although the HfO_{2} films annealed in N_{2}/O_{2} result in lower interface state density and higher channel electron mobility compared to the HfO_{2} films annealed in N_{2}, the determined surface state capture cross-section at the HfO_{2}/Si interface is the same. This suggests that the surface state capture cross-section may be an inherent nature at the interface between silicon and hafnium oxide.

#### Conflict of Interests

The author declares that there is no conflict of interests regarding the publication of this paper.

#### Acknowledgment

The author would like to thank the National Science Council of Taiwan, for supporting this work under Contract no. NSC 102-2221-E-015-MY2.

#### References

- G. D. Wilk, R. M. Wallace, and J. M. Anthony, “High-k gate dielectrics: current status and materials properties considerations,”
*Journal of Applied Physics*, vol. 89, no. 10, pp. 5243–5275, 2001. View at Publisher · View at Google Scholar · View at Scopus - H.-S. P. Wong, H.-Y. Lee, S. Yu et al., “Metal-oxide RRAM,”
*Proceedings of IEEE*, vol. 100, no. 6, pp. 1951–1970, 2012. - Y. H. Wu, D. J. Wouters, P. Hendrickx et al., “On the bipolar resistive switching memory using TiN/Hf/HfO
_{2}/Si MIS structure,”*IEEE Electron Device Letters*, vol. 34, no. 3, pp. 414–416, 2013. - F. Lin, B. Hoex, Y. H. Koh, J. Lin, and A. G. Aberle, “Low-temperature surface passivation of moderately doped crystalline silicon by atomic-layer-deposited hafnium oxide films,”
*ECS Journal of Solid State Science and Technology*, vol. 2, no. 1, pp. N11–N14, 2013. - J. Wang, S. Sadegh Mottaghian, and M. Farrokh Baroughi, “Passivation properties of atomic-layer-deposited hafnium and aluminum oxides on Si surfaces,”
*IEEE Transactions on Electron Devices*, vol. 59, no. 2, pp. 342–348, 2012. View at Publisher · View at Google Scholar · View at Scopus - J. Robertson, “Band offsets of wide-band-gap oxides and implications for future electronic devices,”
*Journal of Vacuum Science and Technology B*, vol. 18, no. 3, pp. 1785–1791, 2000. View at Publisher · View at Google Scholar · View at Scopus - J. McPherson, J.-Y. Kim, A. Shanware, and H. Mogul, “Thermochemical description of dielectric breakdown in high dielectric constant materials,”
*Applied Physics Letters*, vol. 82, no. 13, pp. 2121–2123, 2003. View at Publisher · View at Google Scholar · View at Scopus - K. J. Hubbard and D. G. Schlom, “Thermodynamic stability of binary oxides in contact with silicon,”
*Journal of Materials Research*, vol. 11, no. 11, pp. 2757–2776, 1996. View at Scopus - F.-C. Chiu, “Interface characterization and carrier transportation in metal/HfO
_{2}/silicon structure,”*Journal of Applied Physics*, vol. 100, no. 11, Article ID 114102, 5 pages, 2006. View at Publisher · View at Google Scholar · View at Scopus - A. S. Grove and D. J. Fitzgerald, “Surface effects on
*P-N*junctions: characteristics of surface space-charge regions under non-equilibrium conditions,”*Solid State Electronics*, vol. 9, no. 8, pp. 783–806, 1966. View at Scopus - T. Giebel and K. Goser, “Hot carrier degradation of n-channel MOSFET's characterized by a gated-diode measurement technique,”
*IEEE Electron Device Letter*, vol. 10, no. 2, pp. 76–78, 1989. View at Scopus - S. M. Sze and K. K. Ng,
*Physics of Semiconductor Devices*, John Wiley & Sons, Hoboken, NJ, USA, 3rd edition, 2006. - P. L. Castro and B. E. Doal, “Low-temperature reduction of fast surface states associated with thermally oxidized silicon,”
*Journal of the Electrochemical Society*, vol. 118, no. 2, pp. 280–286, 1971. - P. C. T. Roberts and J. D. E. Beynon, “An experimental determination of the carrier lifetime near the Si-SiO
_{2}interface,”*Solid-State Electronics*, vol. 16, no. 2, pp. 221–227, 1973. View at Scopus - F.-C. Chiu, W.-C. Shih, J. Y.-M. Lee, and H.-L. Hwang, “An investigation of surface state capture cross-sections for metal-oxide-semiconductor field-effect transistors using HfO
_{2}gate dielectrics,”*Microelectronics Reliability*, vol. 47, no. 4-5, pp. 548–551, 2007. View at Publisher · View at Google Scholar · View at Scopus - K. Shiraishi, K. Yamada, K. Torii et al., “Oxygen-vacancy-induced threshold voltage shifts in Hf-related high-k gate stacks,”
*Thin Solid Films*, vol. 508, no. 1-2, pp. 305–310, 2006. View at Publisher · View at Google Scholar · View at Scopus - K. Tse, D. Liu, K. Xiong, and J. Robertson, “Oxygen vacancies in high-k oxides,”
*Microelectronic Engineering*, vol. 84, no. 9-10, pp. 2028–2031, 2007. View at Publisher · View at Google Scholar · View at Scopus - K. Xiong and J. Robertson, “Point defects in HfO
_{2}high K gate oxide,”*Microelectronic Engineering*, vol. 80, pp. 408–411, 2005. View at Publisher · View at Google Scholar · View at Scopus - H. Takeuchi, H. Y. Wong, D. Ha, and T. J. King, “Impact of oxygen vacancies on high-k gate stack engineering,” in
*Proceedings of the 50th IEEE International Electron Devices Meeting (IEDM ’04)*, pp. 829–832, 2004. - S.-I. Takagi, A. Toriumi, M. Iwase, and H. Tango, “On the universality of inversion layer mobility in Si MOSFET's: part I-effects of substrate impurity concentration,”
*IEEE Transactions on Electron Devices*, vol. 41, no. 12, pp. 2357–2362, 1994. View at Publisher · View at Google Scholar · View at Scopus - J. R. Hauser, “Extraction of experimental mobility data for MOS devices,”
*IEEE Transactions on Electron Devices*, vol. 43, no. 11, pp. 1981–1988, 1996. View at Publisher · View at Google Scholar · View at Scopus - D. K. Schroder,
*Semiconductor Material and Device Characterization*, John Wiley & Sons, Hoboken, NJ, USA, 3rd edition, 2006. - P. Masson, J.-L. Autran, and G. Ghibaudo, “An Improved time domain analysis of the charge pumping current,”
*Journal of Non-Crystalline Solids*, vol. 280, no. 1–3, pp. 255–260, 2001. View at Publisher · View at Google Scholar · View at Scopus - G. Groeseneken, H. E. Maes, N. Beltran, and R. F. de Keersmaecker, “A reliable approach to charge-pumping measurements in MOS transistors,”
*IEEE Transactions on Electron Devices*, vol. 31, no. 1, pp. 42–53, 1984. View at Scopus - C.-H. Liu and F.-C. Chiu, “Electrical characterization of ZrO
_{2}/Si interface properties in MOSFETs with ZrO_{2}gate dielectrics,”*IEEE Electron Device Letters*, vol. 28, no. 1, pp. 62–64, 2007. View at Publisher · View at Google Scholar · View at Scopus - P. Saint-Cast, Y. H. Heo, E. Billot et al., “Variation of the layer thickness to study the electrical property of PECVD Al
_{2}O_{3}/c-Si interface,”*Energy Procedia*, vol. 8, pp. 642–647, 2011. - C.-H. Chen, I. Y.-K. Chang, J. Y.-M. Lee, and F.-C. Chiu, “Electrical characterization of CeO
_{2}Si interface properties of metal-oxide-semiconductor field-effect transistors with CeO_{2}gate dielectric,”*Applied Physics Letters*, vol. 92, no. 4, Article ID 043507, 3 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - F.-C. Chiu, S.-Y. Chen, C.-H. Chen, H.-W. Chen, H.-S. Huang, and H.-L. Hwang, “Interfacial and electrical characterization in metal-oxide-semiconductor field-effect transistors with CeO
_{2}gate dielectric,”*Japanese Journal of Applied Physics*, vol. 48, no. 4, Article ID 04C014, 4 pages, 2009. View at Publisher · View at Google Scholar · View at Scopus - J.-P. Han, E. M. Vogel, E. P. Gusev et al., “Energy distribution of interface traps in high-k gated MOSFETs,” in
*Proceedings of the Symposium on VLSI Technology*, pp. 161–162, June 2003. View at Scopus